title: Effects of polishing techniques on the surface roughness of acrylic denture base resins.
abstract: BACKGROUND
  Rough surfaces of denture bases promote adhesion of microorganisms and plaque formation. It is therefore important to know how different polishing systems affect surface roughness of denture base acrylic resins.
  
  
  OBJECTIVE
  The objective of this study was to compare the effects of 4 chairside polishing kits and 2 conventional laboratory techniques used for polishing 3 different acrylic denture base resins.
  
  
  METHODS
  Using contact profilometric measurement, the surface texture of 54 specimens (15x30x3 mm) per acrylic material (autopolymerized ProBase Cold, heat-polymerized ProBase Hot, and injection heat-polymerized SR Ivocap plus) was studied before and after cutting with a tungsten carbide bur, and during and after chairside polishing with 4 polishing kits (Exa Technique, Acrylic Polisher HP blue, AcryPoint, Becht Polishing Cream), and after conventional polishing with 2 polishing systems (Universal Polishing Paste for Resins and Metals, Lesk Polishing Liquid). There were 9 specimens for each acrylic resin material and polishing method combination. Conventional lathe polishing with polishing paste served as the control. Mean average surface roughness (Ra) values of each specimen group were analyzed using a 2-way analysis of variance, the Scheffé post-hoc test, and paired t test (alpha=.05) with the Bonferroni adjustment. After testing the polished acrylic resin surfaces were evaluated under a scanning electron microscope.
  
  
  RESULTS
  The highest mean average surface roughness (Ra=2.86+/-0.8 microm to 3.99+/-1.31 microm) was measured for surfaces finished with a tungsten carbide bur. The lowest surface roughness values (Ra=0.02+/-0.01 microm) were determined for acrylic resin specimens polished with a lathe and polishing paste. The Ra values of resin specimens after polishing with chairside silicone polishing kits ranged from 0.05+/-0.0 microm to 0.35+/-0.05 microm. Mean average Ra values of specimens polished with a polishing cream alone (Ra=1.01+/-0.17 microm to 1.68+/-0.47 microm) were significantly higher (P<.05) than those obtained with other polishing systems tested, which was confirmed by scanning electron microscope images of acrylic resin surfaces. Significant differences in mean average surface roughness were found between autopolymerizing and injected heat-polymerizing resin specimens. In addition, scanning electron microscopy revealed increased porosity of autopolymerizing resin specimens.
  
  
  CONCLUSIONS
  Conventional laboratory polishing was found to produce the smoothest surface of denture base acrylic resin. Chairside silicone polishing kits produced a significantly smoother surface of acrylic resin than specimens polished with a tungsten carbide bur. The presence of large pores was characteristic for the autopolymerizing resin material.
authors.affiliation: University of Ljubljana, Faculty of Medicine, Division of Dental Medicine, Ljubljana, Slovenia. milan.kuhar@mf.uni-lj.si
authors.forename: Milan
authors.initials: M
authors.lastname: Kuhar
authors.forename: Nenad
authors.initials: N
authors.lastname: Funduk
mesh_terms: D000180:Acrylic Resins / Q000737:chemistry*; D003775:Dental Polishing / Q000379:methods*; D003819:Denture Bases; D008855:Microscopy, Electron, Scanning; D013499:Surface Properties
chemical_list: D000180:Acrylic Resins